JOURNAL OF SOLID STATE CHEMISTRY 24, 1-9 (1978)
High-Temperature Thermodynamics of Dilute Solutions of Hydrogen and Deuterium in Tantalum and in Dilute Tantalum-Oxygen Solid Solutions
P. G. DANTZER* AND 0. J. KLEPPAT
The James Franck Institute and The Department of Chemistry, The University of Chicago, Chicago, Illinois 60637
Received July 5, 1977
We report a comparison between the partial enthalpies of solution of hydrogen (dfiu) and of deuterium (&I,) in tantalum at 715OK and find A& - AEi, = -220 caf mole-r. This allows a calculation of the average vibrational frequency of hydrogen which is 1350 cm-r. On the basis of this result we have made a new estimate of the residual excess entropy (ss- &(vibr) - &(el)) for hydrogen and deuterium and find a value of 4.6 cal OK- mole-. This is consistent with occupancy by hydrogen of the tetrahedral interstitial sites, and may possibly reflect occupancy of both tetrahedral and octahedral sites. The presence of oxygen in solid solution in tantalum in amounts of l-3 at.% makes the partial enthalpy of solution more negative, and also reduces the partial entropy by about 1 cal OK-r mole-r. The net effect of these two terms is to increase the partial pressure of hydrogen compared to pure tantalum at low oxygen contents, but to reduce the partial pressure at higher oxygen contents (Nc 2 0.03,).
In recent communications we have pub- lished detailed calorimetric and equilibrium data for the solid solutions of hydrogen in bee V, Nb, and Ta (I, 2). In this work we reported new information on the dependence of the partial enthalpy of solution of hydrogen on temperature, and we attempted to explain the observed values of the excess entropy of hydrogen in terms of vibrational, electronic, volume change, and degeneracy contributions in the manner originally proposed by OKeeffe and Stewart (3).
In our previous calculation of the vibra- tional entropy of hydrogen in tantalum we based our estimate on an assumed vibrational frequency of 970 + 50 cm-, taken from the
l Permanent address: University of Paris&d, Bati- ment 4 15,9 1405 Orsay-Cedex, France.
t Author to whom correspondence is to be addressed.
neutron-scattering work on V-H alloys of Rush and Flotow (4). In the present work we have measured the partial enthalpies of solution of hydrogen and deuterium in tan- talum. This allows us to calculate directly a new average vibrational frequency of hydro- gen, and to obtain a revised value of the vibrational entropy of hydrogen.
A second objective of the present in- vestigation has been the measurement of the partial enthalpy of solution of hydrogen in pure (i.e., as received) tantalum, and in tantalum metal which contained known amounts of oxygen in solid solution. While there have been many thermodynamic in- vestigations of binary metal-hydrogen alloys, we have found very little information in the literature on the thermodynamics of ternary metal-hydrogen-oxygen systems. The present communication represents a modest first ex- ploration in this general area. We propose to
1 0022-4596/78/0241-moMH)1 so2.co/o
Copyright 0 1978 by Academic Press, Inc. All rights of reproduction in any form reserved.
Printed in Great Britain
2 DANTZER AND KLEPPA
give further attention to this problem in future work.
Finally, a third objective of the present work has been to obtain additional information on the fairly reproducible but so far unex- plained anomalies in the observed partial enthalpies and excess entropies of hydrogen in very dilute solutions in tantalum. We observed these anomalies in our earlier work (I, 2), and somewhat similar behavior had previously been reported in equilibrium studies by Kofstad et al. (5), Katz and Gulbransen (6), Veleckis and Edwards (7), and McQuillan and Wallbank (8).
It is not as yet clear to what extent these anomalies might have been caused by the thermal transpiration effect recently discussed by Wallbank and McQuillan (9). However, it was suggested by Kofstad et al., that the anomalies might perhaps be related to the presence in the metal of interstitial impurities such as oxygen, nitrogen, and carbon. In fact, these authors found that the effect was some- what enhanced in experiments on tantalum which contained 0.56 at.% oxygen. We hoped that our own experiments with oxygen- containing alloys might throw some further light on this problem.
Experimental and Materials
Most of our measurements were carried out at 713-716OK using the same gas-measuring system and the same Calvet-type twin calorimeter as in our earlier work. However, for a series of measurements at 876OK we substituted a single unit microcalorimeter suitable for the higher temperature.
The tantalum metal was again in the form of 0.005cm thick foil purchased from Fansteel. However, our sample was taken from a different batch of material. A typical analysis is given in Ref. (I). Prior to use the foil was cut into strips 0.5 cm wide x 7 cm long, degreased in trichlorethylene, and then washed first in acetone and finally in absolute alcohol.
In our study of the solutions of hydrogen and deuterium in pure tantalum, a weighed amount of metal was either enclosed in an 8- cm-long protective stainless steel crucible (to avoid contamination by reaction with the fused silica wall, Series la, lb), or the foil was placed directly into the fused silica liner (Series 2, 3, 4). (Runs labeled by the same serial number used the same weighed-in sample of tantalum. For series denoted by letters, i.e., la, lb, etc., hydrogen was completely desorbed from the sample between runs a and b.)
The alloys of tantalum and oxygen were prepared by dissolving known amounts of oxygen gas in pure tantalum. This process was carried out in the fused silica liner, initiated by heating the liner containing metal and gas at the rate of about 50 per hour from 200 to 600C. At this temperature the initial volume of oxygen gas had been completely absorbed. Finally, the foils were annealed for three days at 950C in order to ensure homogenization of the sample. The oxygen contents of the alloys were checked by the gains in weight, and agreed with the calculated amounts. The following alloy compositions were used: Series 2: Ta, 0.92 at.% 0; Series 3: Ta, 2.97 at.% 0. For these alloy samples we did not use any protective stainless steel crucible between sample and silica liner. However, we prevented direct contact between liner and sample by means of a small silica container.
The hydrogen and deuterium gases were purified by absorption in and desorption from titanium powder. The deuterium gas was purchased from Union Carbide (c.p., -99.5% DJ. As received the tantalum foils react very sluggishly with hydrogen at 700K. In order to obtain acceptable reaction rates the foils were placed in the fused silica liner, and then activated in a separate furnace by absorbing and desorbing purified hydrogen at about 55OOC. This process was repeated four to six times until absorption was essentially instan- taneous. The liner was then evacuated to a pressure of about lO-j Torr while the tem- perature was raised to 640C (Series 1 only)
HYDROGEN IN TANTALUM
l serfes 3 (To,3%0)+H2 0 Series 2 (Ta,l%O)+H2
FIG. 1. Partial enthalpies of solution of hydrogen and of deuterium in tantalum and in tantalum-oxygen solid solutions at indicated temperatures plotted against mole fraction of H(D).
or 850C (all other Series). The sample was maintained at this temperature for about 12 hr before the liner was introduced into the calori- meter.
In order to obtain reasonable heat effects (0.5 cal or larger) and reliable results in the dilute solution range, we used quite large samples of tantalum metal (about 20 g). This has the consequence that for higher hydrogen contents (mole fraction, N, >, 0.06) the amount of gas necessary to produce a signifi- cant change in mole fraction becomes quite large. Also, the time required to reach equilib- rium is longer (> 1 hr), and there is a tendency to underestimate the heat of reaction by perhaps 1 to 2%.
Results and Discussion
The observed partial molar enthalpies of solution of hydrogen are shown graphically in Fig. 1. In comparing our new enthalpy data with our earlier results it should be noted that in our earlier work we incorrectly identified the observed heat effects as changes in internal energy rather than in enthalpy (10). Hence, the previously published enthalpy data are too negative by a term +R T.
Figure 1 shows that for values of NH larger than about 0.02 there is very good agreement between the results obtained in Series la, lb (pretreated at 640C) and Series 4a, 4c (pre- treated at 85OOC). By extrapolating the high- concentration data linearly to NH = 0, we find for these two series the limiting values of dfi, at 713-716OK of -7.73 and -7.65 kcal mole-, respectively. The corresponding value at 703OK taken from Ref. (I) (corrected by +RT) is -7.80 kcal mole-l.
The Isotope Effect In order to obtain the best possible value for
the difference between the enthalpies of solution of hydrogen and of deuterium we carried out four consecutive series of calorimetric measurement on the same metal sample at about 7 15 OK: [4a (Ta + H,); 4b (Ta + DJ; 4c (Ta + H,); 4d (Ta + DJI. The data plotted in Fig. 1 show that there is excellent agreement between the enthalpies measured in Series 4a and 4c on the one hand, and in Series 4b and 4d on the other. We find
AI?, - Al?, = -220 cal mole-
with an estimated uncertainty of about +25 cal
4 DANTZER AND KLEPPA
mole-. This difference applies at all con- centrations up to about NH(u) z 0.06.
It is generally assumed that hydrogen and deuterium dissolved interstitially in metals such as tantalum may be considered as independent, three-dimensional Einstein oscil- lators. If we may also assume that the observed enthalpy difference at 715 OK can be attributed entirely to vibrational effects, we calculate an average vibrational frequency of hydrogen in tantalum of 1350 cm-, with an estimated uncertainty of +50 cm-. Details of this calculation may be found in a recent paper by Dantzer et al. (II).
Note that this frequency is significantly larger than the value, 970 cm-, adopted in our earlier work, which was taken from the neutron-scattering study by Rush and Flotow (4) of hydrogen in vanadium. However, Rush and Flotow also found evidence for another hydrogen frequency of about 1400 cm-, particularly at high hydrogen concentrations.
Last year a new investigation of the localized vibrational modes of hydrogen in tantalum has been published by Yamada et al. (12). These authors studied tantalum- hydrogen alloys of composition TaH,,,, TaHo.Sy and TaH,,, by inelastic neutron scattering at 20 and 85C. At the lower temperature the hydrogen atoms in TaH,,, and TaH,, are ordered; at the higher temperature all alloys are disordered (22).
Yamada et al. confirmed the presence of two hydrogen frequencies at about 970 and 1410 cm-. However, in all cases they found that the integrated intensity of the high energy peak was greater than that of the low energy peak, and also that the relative intensity of the high energy peak increased very considerably on going from 20 to 85~. If we are justified in extrapolating these observations to the very much higher temperature of our calorimetric measurements, we believe our calculated average frequency of 1350 k 50 cm- must be considered to be in very reasonable agreement with Yamada et al.
We are now ready to compare our ex- perimental excess entropies with estimates based on contributions from vibrational, electronic, and degeneracy terms. We define the partial excess entropy of hydrogen through the relation
f?f; = As, + &S& + R In [N,/( 1 - NJ]. (1)
In this expression @& represents the standard entropy of hydrogen gas at the considered temperature, while -R In [lv,/( 1 - NJ repre- sents the ideal (i.e., configurational) partial molar entropy, calculated under the assump- tion that the hydrogen atoms have access to only one interstitial lattice site per tantalum atom.
Our experimental values of Si and Sb are plotted against composition in Fig. 2. We see that our extrapolated experimental value of SE (NH = 0) is 5.4 cal OK-- mole-i; the corre- sponding value of 3: (ND = 0) is 6.8 cal OK- mole-. If we set fin = 1350 cm- and Gn = 1350/~212 = 955 cm-, we calculate at 715OK, S, (vibr) = 1.5 cal OK- mole-, and S, (vibr) = 2.9 cal OK- mole-. The differ- ence between these two values is in excellent agreement with the experimental difference.
Previously we estimated the electronic con- tribution to the partial excess entropy of hydrogen in tantalum near 700K to be -0.7 +_ 0.3 cal OK- mole-. When this estimate is combined with the vibrational terms above and the sums subtracted from Sf; and SE we arrive at a value of 4.6 cal OK- mole- which must be accounted for by other entropy contribu- tions. We believe a major part of this re- sidual entropy must be attributed to the lattice degeneracy of hydrogen on the inter- stitial sites in the bee structure.
It is well known that the bee tantalum structure has six interstitial lattice sites per atom which are tetrahedrally surrounded by tantalum atoms (T sites), and three interstitial sites which are octahedrally coordinated (0 sites).
HYDROGEN IN TANTALUM
I / I 11 I 1 I 1 I 713K A Series la 713K A Series lb Ta+H2
--An- ,Series 40,4c
0.02 0.04 0.06 (208 NH(D)
FIG. 2. Partial excess entropies of hydrogen and of deuterium at indicated temperatures plotted against mole fraction of H(D).
Most of the information presently available on hydrogen site occupancy in body-centered cubic metals is based on neutron-scattering investigations such as the already quoted study by Rush and Flotow (4). Confirming infor- mation has been provided by channeling experiments (13). Most of these studies have been carried out at or near room temperature, and seem to indicate that the hydrogen atoms prefer the T-sites. If this is indeed the case, the site degeneracy contribution to the partial entropy of hydrogen at NH = 0 should be R ln6 = 3.56 cal OK- mole-.
To the best of our knowledge no neutron- scattering study or channeling experiments on Ta + H, or Ta + D, have been carried out at temperatures approaching those of the present investigation. However, if the energy advan- tage of the T-sites compared to the O-sites is not large compared to RT, one might expect the hydrogen atoms to be distributed nearly randomly over both types of sites. In this event a lattice degeneracy term approaching R In 9 = 4.37 cal OK- mole- might be expected.
It will be apparent that both of these values (R ln6 and R ln9), in principle, would be consistent with the observed residual excess entropy of 4.6 cal OK- mole-. However, the value R In 9 would be acceptable only if other excess entropy terms are very small. There are at least two additional contributions which may be significant.
On the one hand, there pres...